#------------------------------------------------------------------------------
#$Date: 2024-04-06 02:40:20 +0300 (Sat, 06 Apr 2024) $
#$Revision: 291107 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/31/24/2312450.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2312450
loop_
_publ_author_name
'Rusanov, Eduard B.'
'Wörle, Michael D'
'Kovalenko, Maksym V.'
'Domasevitch, Kostiantyn V.'
'Rusanova, Julia A.'
_publ_section_title
;
 Attractive and repulsive forces in a crystal of
 [Rb(18-crown-6)][SbCl₆] under high pressure.
;
_journal_issue                   'Pt 2'
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              135
_journal_page_last               145
_journal_paper_doi               10.1107/S2052520624001586
_journal_volume                  80
_journal_year                    2024
_chemical_formula_moiety         'C12 H24 O6 Rb, Cl6 Sb'
_chemical_formula_sum            'C12 H24 Cl6 O6 Rb Sb'
_chemical_formula_weight         684.23
_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_atom_sites_solution_hydrogens   geom
_audit_creation_date             2023-12-19
_audit_creation_method
;
Olex2 1.5
(compiled 2023.03.06 svn.rbb2c1857 for OlexSys, GUI svn.r6748)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   13.7760(8)
_cell_length_b                   13.7760(8)
_cell_length_c                   9.5808(7)
_cell_measurement_pressure       1460000
_cell_measurement_reflns_used    1261
_cell_measurement_temperature    293(1)
_cell_measurement_theta_max      29.0600
_cell_measurement_theta_min      2.6970
_cell_volume                     1574.63(17)
_computing_cell_refinement       'CrysAlisPro 1.171.42.94a (Rigaku OD, 2023)'
_computing_data_collection       'CrysAlisPro 1.171.42.94a (Rigaku OD, 2023)'
_computing_data_reduction        'CrysAlisPro 1.171.42.94a (Rigaku OD, 2023)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_diffrn_ambient_environment      air
_diffrn_ambient_pressure         1460000
_diffrn_ambient_temperature      293(1)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 0.732
_diffrn_measured_fraction_theta_max 0.686
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω     24.00  49.00   1.00    3.00    --   24.80  48.00  95.00   25
  2  ω    -41.00 -19.00   1.00    3.00    --   24.80   0.00  60.00   22
  3  ω    -18.00   5.00   1.00    3.00    --   24.80  57.00 -30.00   23
  4  ω     13.00  38.00   1.00    3.00    --   24.80  33.00 -61.00   25
  5  ω      6.00  31.00   1.00    3.00    --   24.80  58.00 -76.00   25
  6  ω    -33.00  -8.00   1.00    3.00    --   24.80   0.00-150.00   25
  7  ω    -41.00 -19.00   1.00    3.00    --  -26.20   0.00  30.00   22
  8  ω    -39.00 -14.00   1.00    3.00    --  -26.20  77.00 150.00   25
  9  ω     23.00  48.00   1.00    3.00    --  -26.20  48.00  95.00   25
 10  ω      1.00  26.00   1.00    3.00    --  -26.20  33.00 -61.00   25
 11  ω    -28.00   3.00   1.00    3.00    --  -26.20 -19.00-180.00   31
 12  ω    -94.00 -69.00   1.00    3.00    --  -26.20 148.00 -37.00   25
 13  ω    -83.00 -58.00   1.00    3.00    --  -26.20 124.00 157.00   25
 14  ω   -115.00 -74.00   1.00    3.00    --  -26.20-178.00 -90.00   41
 15  ω     -4.00  25.00   1.00    3.00    --  -26.20 -97.00  35.00   29
 16  ω      5.00  33.00   1.00    3.00    --  -26.20-114.00-135.00   28
 17  ω     -4.00  21.00   1.00    3.00    --  -26.20 -97.00-143.00   25
 18  ω     44.00  69.00   1.00    3.00    --   24.80-148.00 -85.00   25
 19  ω     30.00  56.00   1.00    3.00    --   24.80-124.00  78.00   26
 20  ω    -27.00  -2.00   1.00    3.00    --   24.80 -19.00-150.00   25
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Synergy, Dualflex, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_measurement_specimen_support 'diamond anvil cell'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0323417000
_diffrn_orient_matrix_UB_12      -0.0517699000
_diffrn_orient_matrix_UB_13      0.0350971000
_diffrn_orient_matrix_UB_21      -0.0129540000
_diffrn_orient_matrix_UB_22      -0.0285679000
_diffrn_orient_matrix_UB_23      -0.0649133000
_diffrn_orient_matrix_UB_31      0.0481593000
_diffrn_orient_matrix_UB_32      -0.0058555000
_diffrn_orient_matrix_UB_33      0.0061567000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0294
_diffrn_reflns_av_unetI/netI     0.0324
_diffrn_reflns_Laue_measured_fraction_full 0.732
_diffrn_reflns_Laue_measured_fraction_max 0.686
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            2264
_diffrn_reflns_point_group_measured_fraction_full 0.732
_diffrn_reflns_point_group_measured_fraction_max 0.686
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.457
_diffrn_reflns_theta_min         2.727
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    4.408
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.70376
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.94a (Rigaku Oxford Diffraction, 2023)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.165
_exptl_crystal_description       prizm
_exptl_crystal_F_000             1002
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.11
_refine_diff_density_max         0.339
_refine_diff_density_min         -0.375
_refine_diff_density_rms         0.085
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.070
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     42
_refine_ls_number_reflns         553
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.070
_refine_ls_R_factor_all          0.0350
_refine_ls_R_factor_gt           0.0273
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0306P)²+1.2197P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0601
_refine_ls_wR_factor_ref         0.0620
_reflns_Friedel_coverage         0.000
_reflns_number_gt                486
_reflns_number_total             553
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            px5059.cif
_cod_data_source_block           Rb14k6
_cod_depositor_comments
'Adding full bibliography for 2312438--2312457.cif.'
_cod_original_cell_volume        1574.6(2)
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               2312450
_shelx_shelxl_version_number     2018/3
_chemical_oxdiff_formula         C12H24O6RbSbCl6
_chemical_oxdiff_usercomment     'RbCrSbCl6 at 14k6'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.643
_shelx_estimated_absorpt_t_min   0.558
_diffrn_orient_matrix_axis[1]    matrixX
_diffrn_orient_matrix_axis[2]    matrixY
_diffrn_orient_matrix_axis[3]    matrixZ
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups
2. Others
 Fixed Sof: Rb1(0.166667)
3.a Secondary CH2 refined with riding coordinates:
 C1(H1A,H1B), C2(H2A,H2B)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.479
_oxdiff_exptl_absorpt_empirical_full_min 0.779
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Sb1 Sb 0.000000 0.000000 1.000000 0.0231(2) Uani 1 6 d S T P . .
Rb1 Rb 0.000000 0.000000 0.5279(5) 0.0491(13) Uani 0.5 3 d S T P . .
Cl1 Cl 0.08100(8) 0.16186(8) 0.85568(10) 0.0374(3) Uani 1 1 d . . . . .
O1 O 0.06396(19) 0.2300(2) 0.4741(2) 0.0280(6) Uani 1 1 d . . . . .
C1 C 0.1759(3) 0.3057(3) 0.5194(4) 0.0293(9) Uani 1 1 d . . . . .
H1A H 0.179447 0.306429 0.620529 0.035 Uiso 1 1 calc R U . . .
H1B H 0.198875 0.380966 0.487590 0.035 Uiso 1 1 calc R U . . .
C2 C 0.2526(3) 0.2681(3) 0.4602(4) 0.0284(8) Uani 1 1 d . . . . .
H2A H 0.240921 0.256714 0.360342 0.034 Uiso 1 1 calc R U . . .
H2B H 0.330059 0.325142 0.476231 0.034 Uiso 1 1 calc R U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_axis.id
_axis.type
_axis.equipment
_axis.parity
_axis.depends_on
_axis.zero
_axis.vector[1]
_axis.vector[2]
_axis.vector[3]
source . source . . . 0.99999993 0.00000000 0.00038642
omega rotation goniometer -1 . -0.36958000 0.00000000 0.00000000 1.00000000
kappa rotation goniometer -1 omega -0.12491000 -0.76551937 0.00000000 0.64341284
phi rotation goniometer -1 kappa . -0.00006597 0.00000000 1.00000000
theta rotation goniometer -1 . 0.65160000 0.00000000 0.00000000 1.00000000
matrixX general general . phi . 1.00000000 0.00000000 0.00000000
matrixY general general . phi . 0.00000000 1.00000000 0.00000000
matrixZ general general . phi . 0.00000000 0.00000000 1.00000000
dacX translation general . phi . 0.00000000 1.00000000 0.00000000
dacY translation general . phi . -1.00000000 0.00000000 0.00000000
dacZ translation general . phi . 0.00000000 0.00000000 1.00000000
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Cl1 Sb1 Cl1 180.00(4) 11_557 2 ?
Cl1 Sb1 Cl1 89.52(3) 12_557 10_557 ?
Cl1 Sb1 Cl1 89.52(3) 3 . ?
Cl1 Sb1 Cl1 89.52(3) 11_557 12_557 ?
Cl1 Sb1 Cl1 89.52(3) 2 . ?
Cl1 Sb1 Cl1 90.48(3) 2 12_557 ?
Cl1 Sb1 Cl1 90.48(3) 2 10_557 ?
Cl1 Sb1 Cl1 90.48(3) 11_557 3 ?
Cl1 Sb1 Cl1 90.48(3) 3 10_557 ?
Cl1 Sb1 Cl1 89.52(3) 2 3 ?
Cl1 Sb1 Cl1 90.48(3) 12_557 . ?
Cl1 Sb1 Cl1 180.00(4) 12_557 3 ?
Cl1 Sb1 Cl1 180.0 10_557 . ?
Cl1 Sb1 Cl1 89.52(3) 11_557 10_557 ?
Cl1 Sb1 Cl1 90.48(3) 11_557 . ?
O1 Rb1 Cl1 68.86(8) 11_556 . ?
O1 Rb1 Cl1 120.86(12) 2 . ?
O1 Rb1 Cl1 69.71(7) . . ?
O1 Rb1 Cl1 120.87(14) 10_556 . ?
O1 Rb1 Cl1 106.91(10) 3 . ?
O1 Rb1 Cl1 82.24(9) 12_556 . ?
O1 Rb1 O1 169.31(19) 10_556 . ?
O1 Rb1 O1 169.31(19) 12_556 3 ?
O1 Rb1 O1 60.453(17) 12_556 . ?
O1 Rb1 O1 116.87(6) 3 . ?
O1 Rb1 O1 60.454(17) 11_556 . ?
O1 Rb1 O1 60.451(17) 12_556 2 ?
O1 Rb1 O1 119.993(3) 11_556 10_556 ?
O1 Rb1 O1 169.31(19) 11_556 2 ?
O1 Rb1 O1 60.451(17) 11_556 3 ?
O1 Rb1 O1 60.455(17) 10_556 2 ?
O1 Rb1 O1 119.996(3) 12_556 10_556 ?
O1 Rb1 O1 116.88(6) 3 2 ?
O1 Rb1 O1 119.997(3) 12_556 11_556 ?
O1 Rb1 O1 116.87(6) . 2 ?
O1 Rb1 O1 60.452(17) 10_556 3 ?
Sb1 Cl1 Rb1 94.02(5) . . ?
C1 O1 Rb1 115.9(2) . 10_556 ?
C1 O1 Rb1 111.9(2) . . ?
C2 O1 Rb1 113.9(2) 12_556 10_556 ?
C2 O1 Rb1 108.4(2) 12_556 . ?
C2 O1 C1 111.9(3) 12_556 . ?
O1 C1 H1A 109.9 . . ?
O1 C1 H1B 109.9 . . ?
O1 C1 C2 108.8(3) . . ?
H1A C1 H1B 108.3 . . ?
C2 C1 H1A 109.9 . . ?
C2 C1 H1B 109.9 . . ?
O1 C2 C1 109.2(3) 11_556 . ?
O1 C2 H2A 109.8 11_556 . ?
O1 C2 H2B 109.8 11_556 . ?
C1 C2 H2A 109.8 . . ?
C1 C2 H2B 109.8 . . ?
H2A C2 H2B 108.3 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sb1 Cl1 2.3750(9) 11_557 ?
Sb1 Cl1 2.3750(9) 10_557 ?
Sb1 Cl1 2.3750(9) 3 ?
Sb1 Cl1 2.3750(9) 2 ?
Sb1 Cl1 2.3750(9) . ?
Sb1 Cl1 2.3750(9) 12_557 ?
Rb1 Rb1 0.534(10) 10_556 ?
Rb1 Cl1 3.687(4) . ?
Rb1 O1 2.832(3) 12_556 ?
Rb1 O1 2.879(3) . ?
Rb1 O1 2.879(3) 2 ?
Rb1 O1 2.832(3) 11_556 ?
Rb1 O1 2.832(3) 10_556 ?
Rb1 O1 2.879(3) 3 ?
O1 C1 1.430(4) . ?
O1 C2 1.425(4) 12_556 ?
C1 H1A 0.9700 . ?
C1 H1B 0.9700 . ?
C1 C2 1.501(6) . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Rb1 O1 C1 C2 51.1(3) . . . . ?
Rb1 O1 C1 C2 40.2(4) 10_556 . . . ?
O1 C1 C2 O1 -69.3(4) . . . 11_556 ?
C2 O1 C1 C2 173.0(3) 12_556 . . . ?
